#------------------------------------------------------------------------------
#$Date: 2019-11-22 22:24:58 +0200 (Fri, 22 Nov 2019) $
#$Revision: 231424 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/00/31/4003195.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4003195
loop_
_publ_author_name
'McKellar, Scott C.'
'Sotelo, Jorge'
'Greenaway, Alex'
'Mowat, John P. S.'
'Kvam, Odin'
'Morrison, Carole A.'
'Wright, Paul A.'
'Moggach, Stephen A.'
_publ_section_title
;
 Pore Shape Modification of a Microporous Metal--Organic Framework Using
 High Pressure: Accessing a New Phase with Oversized Guest Molecules
;
_journal_issue                   2
_journal_name_full               'Chemistry of Materials'
_journal_page_first              466
_journal_paper_doi               10.1021/acs.chemmater.5b02891
_journal_volume                  28
_journal_year                    2016
_chemical_formula_moiety         'C30 H12 O12 Sc2'
_chemical_formula_sum            'C30 H12 O12 Sc2'
_chemical_formula_weight         654.33
_space_group_IT_number           70
_space_group_name_Hall           '-F 2uv 2vw'
_space_group_name_H-M_alt        'F d d d :2'
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      70
_symmetry_space_group_name_Hall  '-F 2uv 2vw'
_symmetry_space_group_name_H-M   'F d d d :2'
_atom_sites_solution_hydrogens   difmap
_atom_sites_solution_primary     other
_audit_creation_date             15-06-08
_audit_creation_method           CRYSTALS_ver_14.40
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.7373(15)
_cell_length_b                   20.691(2)
_cell_length_c                   34.124(6)
_cell_measurement_reflns_used    1609
_cell_measurement_temperature    293
_cell_measurement_theta_max      17
_cell_measurement_theta_min      4
_cell_volume                     6169.1(16)
_computing_cell_refinement       'Apex2 (Bruker AXS, 2006)'
_computing_data_collection       'Apex2 (Bruker AXS, 2006)'
_computing_data_reduction        'Apex2 (Bruker AXS, 2006)'
_computing_molecular_graphics    'CAMERON (Watkin et al., 1996)'
_computing_publication_material  'CRYSTALS (Betteridge et al., 2003)'
_computing_structure_refinement  'CRYSTALS (Betteridge et al., 2003)'
_computing_structure_solution    'Superflip (Palatinus & Chapuis, 2007)'
_diffrn_ambient_pressure         400000
_diffrn_ambient_temperature      293
_diffrn_measured_fraction_theta_full 0.735
_diffrn_measured_fraction_theta_max 0.726
_diffrn_measurement_device       Area
_diffrn_measurement_device_type  'Bruker Kappa Apex2'
_diffrn_measurement_method       ω
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.070
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_number            2228
_diffrn_reflns_theta_full        14.969
_diffrn_reflns_theta_max         16.632
_diffrn_reflns_theta_min         3.811
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    0.501
_exptl_absorpt_correction_T_max  0.95
_exptl_absorpt_correction_T_min  0.75
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Siemens, 1996)'
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    1.409
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             2640
_exptl_crystal_size_max          0.200
_exptl_crystal_size_mid          0.150
_exptl_crystal_size_min          0.100
_refine_diff_density_max         0.61
_refine_diff_density_min         -0.58
_refine_ls_extinction_coef       8.524
_refine_ls_extinction_method     'Larson (1970), Equation 22'
_refine_ls_goodness_of_fit_ref   1.0247
_refine_ls_hydrogen_treatment    noref
_refine_ls_matrix_type           full
_refine_ls_number_parameters     87
_refine_ls_number_reflns         304
_refine_ls_number_restraints     83
_refine_ls_R_factor_all          0.0942
_refine_ls_R_factor_gt           0.0744
_refine_ls_shift/su_max          0.0339588
_refine_ls_shift/su_mean         0.0017951
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
;
 Method= Modified Sheldrick 
 w=1/[σ²(F²) + ( 0.00P)² +*****P] 
 ,where P=(max(Fo²,0) + 2Fc²)/3 
;
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_all         0.1741
_refine_ls_wR_factor_gt          0.1658
_refine_ls_wR_factor_ref         0.1741
_reflns_limit_h_max              6
_reflns_limit_h_min              0
_reflns_limit_k_max              16
_reflns_limit_k_min              0
_reflns_limit_l_max              23
_reflns_limit_l_min              0
_reflns_number_gt                244
_reflns_number_total             308
_reflns_threshold_expression     I>2.0σ(I)
_oxford_diffrn_Wilson_B_factor   0.00
_oxford_diffrn_Wilson_scale      0.00
_oxford_refine_ls_r_factor_ref   0.0942
_oxford_refine_ls_scale          0.04991(6)
_oxford_reflns_number_all        304
_oxford_reflns_threshold_expression_ref I>-3.0\s(I)
_oxford_structure_analysis_title 'ST3132s in Fddd'
_cod_data_source_file            cm5b02891_si_003.cif
_cod_data_source_block           SC2BDC3_23dmb_II
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_atom_sites_solution_primary' value 'Other' was changed to
'other' in accordance with the
/home/saulius/struct/COD-crude-data/automatic-downloads/DataCite-retrospective/ACS/depositions/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

Automatic conversion script
Id: cif_fix_values 6909 2019-04-08 15:41:33Z antanas 
;
_cod_original_cell_volume        6169.1(17)
_cod_original_sg_symbol_H-M      'F d d d'
_cod_database_code               4003195
_iucr_refine_instruction_details_constraints
;
#
# Punched on 08/06/15 at 11:59:00
#
#LIST     12                                                                    
BLOCK 
CONT SCALE 
CONT SC   (1 ,X'S,U'S)  UNTIL C(4) 
CONT C (5, X'S,U[ISO]) UNTIL C(8) 
CONT C (9, X'S,U[ISO]) UNTIL C(10) 
END                                                                             
;
_iucr_refine_instruction_details_restraints
;
#
# Punched on 08/06/15 at 11:59:00
#
#LIST     16                                                                    
NO 
DIST 1.39, 0.01 = C(2) TO C(3) 
DIST 1.39, 0.01 = C(3) TO C(4) 
DIST 1.39, 0.01 = C(2,-1,4,0,0,1) TO C(4) 
DIST 1.39, 0.01 = C(6) TO C(7) 
DIST 1.39, 0.01 = C(7) TO C(8) 
DIST 1.39, 0.01 = C(8) TO C(6,-2,1,0,1,1) 
ANGLE 120, 1 = C(2) TO C(3) TO C(4) 
ANGLE 120, 1 = C(1) TO C(2) TO C(3) 
ANGLE 120, 1 = C(4,-1,4,0,0,1) TO C(2) TO C(3) 
ANGLE 120, 1 = C(7) TO C(8) TO C(6,-2,1,0,1,1) 
ANGLE 120, 1 = C(6) TO C(7) TO C(8) 
ANGLE 120, 1 = C(5) TO C(6) TO  C(7) 
PLANAR 0.010000  C(6) C(7) C(8)  C(6,-2,1,0,1,1) 
PLANAR 0.010000  C(2,-1,4,0,0,1) C(2) C(3) C(4) 
REM   DELU   START (DO NOT REMOVE THIS LINE) 
VIBR .0, 0.00200 = O(1) TO C(1) 
VIBR .0, 0.00200 = O(2) TO C(1) 
VIBR .0, 0.00200 = O(3) TO C(5) 
VIBR .0, 0.00200 = C(1) TO C(2) 
VIBR .0, 0.00500 = O(1) TO O(2) 
VIBR .0, 0.00500 = C(2) TO O(2) 
VIBR .0, 0.00500 = C(2) TO O(1) 
VIBR .0, 0.00200 = C(2) TO C(4,-1,4,0,0,1) 
VIBR .0, 0.00200 = C(2) TO C(3) 
VIBR .0, 0.00500 = C(4,-1,4,0,0,1) TO C(1) 
VIBR .0, 0.00500 = C(3) TO C(1) 
VIBR .0, 0.00500 = C(3) TO C(4,-1,4,0,0,1) 
VIBR .0, 0.00200 = C(3) TO C(4) 
VIBR .0, 0.00500 = C(4) TO C(2) 
VIBR .0, 0.00500 = C(2,-1,4,0,0,1) TO C(3) 
VIBR .0, 0.00200 = C(5) TO C(6) 
VIBR .0, 0.00500 = O(3,-3,1,0,0,1) TO O(3) 
VIBR .0, 0.00500 = C(6) TO O(3) 
VIBR .0, 0.00500 = C(6) TO O(3,-3,1,0,0,1) 
VIBRATION 0.0, 0.020000 = C(6) TO C(7) 
VIBRATION 0.0, 0.020000 = C(7) TO C(8) 
VIBRATION 0.0, 0.050000 = C(6) TO C(8) 
VIBRATION 0.0, 0.050000 = C(5) TO C(7) 
REM   DELU   END (DO NOT REMOVE THIS LINE) 
REM   THERMSIM   START (DO NOT REMOVE THIS LINE) 
U(IJ) .0, 0.08000 = O(1) TO C(1) 
U(IJ) .0, 0.08000 = O(2) TO C(1) 
U(IJ) .0, 0.04000 = O(3) TO C(5) 
U(IJ) .0, 0.04000 = C(1) TO C(2) 
U(IJ) .0, 0.04000 = C(2) TO C(4,-1,4,0,0,1) 
U(IJ) .0, 0.04000 = C(2) TO C(3) 
U(IJ) .0, 0.04000 = C(3) TO C(4) 
U(IJ) .0, 0.04000 = C(5) TO C(6) 
U(IJ)'S  0.0, 0.010000 = C(7) TO C(8) 
U(IJ)'S  0.0, 0.010000 = C(6) TO C(7) 
REM   THERMSIM   END (DO NOT REMOVE THIS LINE) 
DISTANCE 1.490000 , 0.010000 = C(9) TO C(10) 
DISTANCE 1.490000 , 0.010000 = C(10) TO C(10,-3,1,1) 
ANGLE 113.000000 , 1.000000 = C(9) TO C(10) TO C(10,-3,1,1) 
ANGLE 113.000000 , 1.000000 = C(9) TO C(10) TO C(10,4,2,1,-1,-1) 
VIBRATION 0.0, 0.020000 = C(9) TO C(10) 
U(IJ)'S  0.0, 0.010000 = C(9) TO C(10) 
END                                                                             
;
loop_
_symmetry_equiv_pos_as_xyz
x,y,z
-x,-y,-z
x,y+1/2,z+1/2
-x,-y+1/2,-z+1/2
x+1/2,y,z+1/2
-x+1/2,-y,-z+1/2
x+1/2,y+1/2,z
-x+1/2,-y+1/2,-z
-x,y+1/4,z+1/4
x,-y+1/4,-z+1/4
-x,y+3/4,z+3/4
x,-y+3/4,-z+3/4
-x+1/2,y+1/4,z+3/4
x+1/2,-y+1/4,-z+3/4
-x+1/2,y+3/4,z+1/4
x+1/2,-y+3/4,-z+1/4
x+1/4,-y,z+1/4
-x+1/4,y,-z+1/4
x+1/4,-y+1/2,z+3/4
-x+1/4,y+1/2,-z+3/4
x+3/4,-y,z+3/4
-x+3/4,y,-z+3/4
x+3/4,-y+1/2,z+1/4
-x+3/4,y+1/2,-z+1/4
-x+1/4,-y+3/4,z+1/2
x+1/4,y+3/4,-z+1/2
-x+1/4,-y+5/4,z+1
x+1/4,y+5/4,-z+1
-x+3/4,-y+3/4,z+1
x+3/4,y+3/4,-z+1
-x+3/4,-y+5/4,z+1/2
x+3/4,y+5/4,-z+1/2
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_occupancy
_atom_site_adp_type
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
Sc1 Sc 0.3750 0.3750 0.63578(13) 0.0192 1.0000 Uani S T
O1 O 0.2442(15) 0.3352(6) 0.5930(4) 0.0523 1.0000 Uani . U
O2 O 0.0070(15) 0.3334(6) 0.5704(3) 0.0432 1.0000 Uani . U
O3 O 0.2469(15) 0.4574(5) 0.6363(4) 0.0625 1.0000 Uani . U
C1 C 0.148(3) 0.3198(9) 0.5673(6) 0.0430 1.0000 Uani D U
C2 C 0.2001(13) 0.2845(3) 0.5328(2) 0.0449 1.0000 Uani D U
C3 C 0.0956(10) 0.2636(4) 0.5051(3) 0.0605 1.0000 Uani D U
C4 C 0.1461(14) 0.2291(4) 0.4726(3) 0.0631 1.0000 Uani D U
C5 C 0.1250 0.4833(11) 0.6250 0.042(6) 1.0000 Uiso DS U
C6 C 0.1250 0.5578(5) 0.6250 0.042(6) 1.0000 Uiso DS U
C7 C 0.2504(10) 0.5913(5) 0.6396(2) 0.052(10) 0.5000 Uiso D U
C8 C 0.2503(10) 0.6586(5) 0.6396(3) 0.067(11) 0.5000 Uiso D U
C9 C 0.595(16) 0.1900(14) 0.0863(6) 0.73(8) 1.0000 Uiso D U
C10 C 0.6250 0.1250 0.10319(13) 0.72(8) 1.0000 Uiso DS U
H31 H -0.0103 0.2727 0.5083 0.0728 1.0000 Uiso . .
H41 H 0.0738 0.2146 0.4537 0.0758 1.0000 Uiso . .
H71 H 0.3280 0.5686 0.6534 0.0625 0.5000 Uiso . .
H81 H 0.3279 0.6812 0.6534 0.0804 0.5000 Uiso . .
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_Cromer_Mann_a1
_atom_type_scat_Cromer_Mann_b1
_atom_type_scat_Cromer_Mann_a2
_atom_type_scat_Cromer_Mann_b2
_atom_type_scat_Cromer_Mann_a3
_atom_type_scat_Cromer_Mann_b3
_atom_type_scat_Cromer_Mann_a4
_atom_type_scat_Cromer_Mann_b4
_atom_type_scat_Cromer_Mann_c
_atom_type_scat_source
C 0.0033 0.0016 2.3100 20.8439 1.0200 10.2075 1.5886 0.5687 0.8650 51.6512
0.2156 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
H 0.0000 0.0000 0.4930 10.5109 0.3229 26.1257 0.1402 3.1424 0.0408 57.7998
0.0030 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
O 0.0106 0.0060 3.0485 13.2771 2.2868 5.7011 1.5463 0.3239 0.8670 32.9089
0.2508 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
Sc 0.2519 0.3716 9.1890 9.0213 7.3679 0.5729 1.6409 136.1080 1.4680 51.3531
1.3329 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_site_symmetry_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
O2 16_556 Sc1 O2 18_556 87.8(7) yes
O2 16_556 Sc1 O3 29_554 92.1(5) yes
O2 18_556 Sc1 O3 29_554 87.3(5) yes
O2 16_556 Sc1 O1 29_554 92.1(5) yes
O2 18_556 Sc1 O1 29_554 179.3(5) yes
O3 29_554 Sc1 O1 29_554 92.1(5) yes
O2 16_556 Sc1 O1 . 179.3(5) yes
O2 18_556 Sc1 O1 . 92.1(5) yes
O3 29_554 Sc1 O1 . 88.6(5) yes
O1 29_554 Sc1 O1 . 88.0(8) yes
O2 16_556 Sc1 O3 . 87.3(5) yes
O2 18_556 Sc1 O3 . 92.1(5) yes
O3 29_554 Sc1 O3 . 179.1(8) yes
O1 29_554 Sc1 O3 . 88.6(5) yes
O1 . Sc1 O3 . 92.1(5) yes
Sc1 . O1 C1 . 169.3(15) yes
Sc1 16_456 O2 C1 . 133.8(12) yes
Sc1 . O3 C5 . 145.3(13) yes
O2 . C1 O1 . 122(2) yes
O2 . C1 C2 . 118.8(14) yes
O1 . C1 C2 . 118.8(18) yes
C1 . C2 C4 8_556 120.9(10) yes
C1 . C2 C3 . 120.1(8) yes
C4 8_556 C2 C3 . 119.0(7) yes
C2 . C3 C4 . 119.7(7) yes
C2 . C3 H31 . 120.1 no
C4 . C3 H31 . 120.1 no
C3 . C4 C2 8_556 121.2(9) yes
C3 . C4 H41 . 119.4 no
C2 8_556 C4 H41 . 119.4 no
O3 . C5 O3 18_556 129(2) yes
O3 . C5 C6 . 115.3(11) yes
O3 18_556 C5 C6 . 115.3(11) yes
C5 . C6 C8 10_566 120.1(6) yes
C5 . C6 C8 27_554 120.1(6) yes
C8 10_566 C6 C8 27_554 119.9(13) yes
C5 . C6 C7 18_556 120.0(5) yes
C8 10_566 C6 C7 18_556 104.0(8) yes
C8 27_554 C6 C7 18_556 42.1(5) yes
C5 . C6 C7 . 120.0(5) yes
C8 10_566 C6 C7 . 42.1(5) yes
C8 27_554 C6 C7 . 104.0(8) yes
C7 18_556 C6 C7 . 120.1(10) yes
C6 . C7 C7 10_566 101.3(6) yes
C6 . C7 C8 10_566 69.0(7) yes
C7 10_566 C7 C8 10_566 54.2(8) yes
C6 . C7 C8 . 119.9(7) yes
C7 10_566 C7 C8 . 35.6(6) yes
C8 10_566 C7 C8 . 89.8(12) yes
C6 . C7 H71 . 119.6 no
C7 10_566 C7 H71 . 133.7 no
C8 10_566 C7 H71 . 119.8 no
C8 . C7 H71 . 119.7 no
C7 . C8 C6 10_566 120.1(8) yes
C7 . C8 C8 10_566 35.7(5) yes
C6 10_566 C8 C8 10_566 101.4(7) yes
C7 . C8 C7 10_566 90.2(12) yes
C6 10_566 C8 C7 10_566 68.9(7) yes
C8 10_566 C8 C7 10_566 54.4(9) yes
C7 . C8 H81 . 119.5 no
C6 10_566 C8 H81 . 119.5 no
C8 10_566 C8 H81 . 133.7 no
C7 10_566 C8 H81 . 119.7 no
C10 18_655 C10 C9 27_644 112.8(8) yes
C10 18_655 C10 C9 . 112.8(8) yes
C9 27_644 C10 C9 . 134.4(17) yes
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Sc1 O2 16_556 2.076(12) yes
Sc1 O2 18_556 2.076(12) yes
Sc1 O3 29_554 2.039(11) yes
Sc1 O1 29_554 2.028(13) yes
Sc1 O1 . 2.028(13) yes
Sc1 O3 . 2.039(11) yes
O1 C1 . 1.26(2) yes
O2 C1 . 1.27(2) yes
O3 C5 . 1.253(13) yes
C1 C2 . 1.46(2) yes
C2 C4 8_556 1.385(8) yes
C2 C3 . 1.385(8) yes
C3 C4 . 1.392(8) yes
C3 H31 . 0.950 no
C4 H41 . 0.950 no
C5 C6 . 1.54(2) yes
C6 C8 10_566 1.390(8) yes
C6 C8 27_554 1.390(8) yes
C6 C7 18_556 1.390(8) yes
C6 C7 . 1.390(8) yes
C7 C7 10_566 1.715(19) yes
C7 C8 10_566 0.999(13) yes
C7 C8 . 1.391(8) yes
C7 H71 . 0.950 no
C8 C8 10_566 1.71(2) yes
C8 H81 . 0.950 no
C9 C10 . 1.487(9) yes
C10 C10 18_655 1.489(9) yes
loop_
_oxford_refln_omitted_index_h
_oxford_refln_omitted_index_k
_oxford_refln_omitted_index_l
_oxford_refln_omitted_flag
3 7 19 x
